Mataqi, K.Y. , Akbar, B.H. / International Journal of Engineering Research and Applications(IJERA) ISSN: 2248-9622 www.ijera.comVol. 3, Issue 2, March -April 2013, pp.617-623617 | P a g eSulfur cycle of microbial corrosion on carbon steel in soil modelMataqi, K.Y. *, Akbar, B.H.***(Department of Biotechnology, Kuwait Institute for Scientific Research, Kuwait)** (Department of Biotechnology Kuwait Institute for Scientific Research, Kuwait)ABSTRACTThis study examined the effects ofDesulfovibrio desulfricans and bacteria consortiaon the rate of carbon steel corrosion in soil model.Microbial corrosion was measured using thecorroded mean depth after 56 days incubationunder aerobic and anaerobic conditions. Theeffects of water content and dissolved oxygen insoil on the corrosion rate were also analyzed.Results showed that aerobic conditions increasedcorrosion rate. Moreover, sole Desulfovibriodesulfricans treatment ceased the corrosion as aprotective ferrous sulfide film formed on thecarbon steel. While the heterogeneous biofilm ofthe bacterial consortia formed uneven oxygenconcentration which accelerated the corrosion.Keywords - Bacteria , Carbon steel, Corrosion,SRB, Desulfovibrio desulfricansI. IntroductionCorrosion is an ever-present degradation mechanismin wetted components and systems. There are manyforms of corrosion in metals, that include; pitting,stress corrosion, general corrosion, galvaniccorrosion, and others , in which microbiologisthave recognized and are constantly addressing.When a system`first encounters microbial corrosion(MC) such event usually occurs during the systeminitial exposure to an aqueous environment, such asduring hydrotest, wet lay-up, or moist soil. Thepresence of certain bacteria in an environment willlead to the production of microbial corrosions. Thismode of corrosion can be accelerated by microbialorganisms, either because they manufactureaggressive species, such as protons or sulphide ions,or because they catalyze the electrochemicalreactions themselves . MC induction also requiresthe presence of nutrients and water to ensure thesurvival and growth of microorganisms. Thus, theability of microorganisms to sense and rapidlyresponse to harsh environmental changes is vital fortheir survival and MC capabilities . Microbes cangrow in fluids with pH values ranging from -1 to 10,where -1 is the most acidic concentration, and deriveenergy from organic or inorganic materials.Moreover, microbes can survive temperatures whichrange from -4 to 210oF (-20 to 99oC) . Themajority of the active organisms involved incorrosion are bacteria, about 1-5 micrometers long,which either oxidize or reduce sulphur compounds assome part of their life process. Although manyculturable bacterial types with known corrosioneffects have been identified , in both aquatic andterrestrial environments the primary corrosion-causing bacteria are the sulfate-reducing iron-oxidizing bacteria. Desulfovibrio desulfricans isexamined in this report as a source of Sulfatereducers, which is found to exist in all soil and watertypes, as well as lives symbiotically with facultativeanaerobic bacteria . Sulfate-reducing bacteria(SRB) are a group of anaerobic diverse organisms inwhich have varied morphological and nutritionalcharacteristics. They utilize organic matter to producesulfide by either reducing or oxidizing sulfatecompounds  , as a source of energy. Therefore,sulphate (SO42–) can be reduced to sulphide (S2–) bySRB leading to the generation of hydrogen sulfide asa metabolic bi-product. Both physical and chemicalprocesses transfer Hydrogen sulfide (H2S) across theair and water boundaries to environments wherechemoautotrophic bacteria oxidize the sulfide tosulfuric acid . The corrosion process will henceoccur by the reaction of the biogenic sulfuric acidwith the metallic surfaces . In order to evaluate thesignificance of microbial corrosions, a look at theeconomical perspective on such effects is essential.In 2001, the cost of microbial-influenced corrosionon oil and gas industries accounted for about $2billion annually . Microbial induced corrosion inthe US economy has reached $350 billion annually asof 2010 . Mild steel in used widely in pipingsystems, storage tanks, cooling towers and aquaticstructures and is the most readily corroded metals. Since bacteria form colonies beneath whichcorrosion can occur, prevention of colonization is oneof the potential ways to prevent MC. This report willexamine the effects of Desulfovibrio desulfricans andbacteria consortia on the rate of carbon steelcorrosion in soil model with respect to dissolvedoxygen and water content distribution in such asystem.II. Materials and Methods2.1 OrganismsThe sulfate reducing bacterial stainDesulfovibrio desulfricans DSMZ 642 was used asthe model SRB in this study. Activated sludge from amunicipal wastewater plant was used as modelBacteria consortia.
Mataqi, K.Y. , Akbar, B.H. / International Journal of Engineering Research and Applications(IJERA) ISSN: 2248-9622 www.ijera.comVol. 3, Issue 2, March -April 2013, pp.617-623618 | P a g e2.2 Culture mediumModified Baar`s Medium (MBM), containing (ing/L) anhydrous sodium citrate 5.0, 50% sodiumlactate 4.9, yeast extract 1.0, NH4Cl 1.0,MgSO4.7H2O 2.0, CaSO4 1.0, and K2HPO4 0.5, wasused as culture medium. The pH, sulfateconcentration and total organic carbon concentration(TOC) of MBM are 7.0, 1500 mg/L, and 2500 mg/L,respectively. SRB and activated sludge were pre-incubated in MBM at 37oC and 25oC, respectively,for seven days. Then, one-tenth of these pre-incubated culture broths were inoculated into testculture medium. The inoculated SRB size was 4x105colony forming unit (CFU) CFU/mL D. desulfricansand 3x107CFU/mL facultative anaerobic bacteria.The inoculated activated sludge size was 7500mg/Lmixed liquor suspended solid (MLSS). Sterile MBMwas prepared by autoclaving the medium at 120̊ C for20min.2.3 Carbon steel coupons preparationRectangular carbon steel coupons (20x10mm and0.35mm thick) were cut from a sheet stock. Thecomposition of the carbon steel coupons was (in wt%) 99.71 Fe, 0.03 C, 0.01 Si, 0.19 Mn, 0.013 P,0.017 S, 0.0017 N, and 0.026Al. The surface waswet-polished with 800-grid polishing paper. Thepolished coupons were cleaned ultrasonically inacetone for 15min, weighed, air-dried, and stored in adesecrator.2.4 Corrosion MeasurementsThe corroded mean depth (CMD) was used as anindicator of the extent of corrosion. Corrosionproducts were selectively removed from testedcoupons by incubating at 60oC for 60 min in a 10wt%HCl solution with 0.3vol% Ibit, a polycationic aminederivative that protects metal steel surface from HCl.Then the treated coupons were weighed. Mass lossof the carbon steel coupon was divided by thespecific gravity of iron (7.86g/cm3) and by the area(cm2) of the carbon steel coupon, and CMD wasderived.2.5 Model soil preparationFigure 1. Experimental apparatuses for preparation ofartificial model soil. (A) Anaerobic conditions: (1)30mL vial bottle; (2) butyl rubber plug; (3) aluminumcap; (4) Na2S solution in 500µL microtube; (5)carbon steel coupons; (6) culture medium in SiO2soil. (B) Aerobic conditions: (7) 50mL centrifugetube; (8) silicone plug.To create artificial model soil, 30mL vials (NichidenRika Garasu, Hyogo) containing 25g silicon dioxide(SiO2) sand, a 500µL microtube, and three carbonsteel coupons were autoclaved, sealed with a butylrubber plug and an aluminum cap, and replaced withN2 gas (N2 >99.9995%) (Figure, 1A). To maintainthe anaerobic conditions throughout the experiment,400µL of 27.2g/L Na2S solution was poured into themicrotube. Then, 7.5mL of the degassed culturemedium was inoculated. To maintain aerobicconditions, a 50mL centrifuge tube containing 25gSiO2 and three carbon steel coupons was autoclaved.Followed by the inoculation with 7.5mL of theculture medium (Fig, 1B).2.6 Measurement of water content on corrosionTo investigate the effects of water content oncorrosion, 4.5 or 1.5mL culture medium wasinoculated. Water content (WC) was defined as theratio of water volume to void of the model soil.Since the void of 25g SiO2 7.5mL, addition of 7.5,4.5 and 1.5mL of culture medium resulted in 100, 60and 20% WC, respectively. To keep the waterconstant in the test tube, sterile water was added andthe tube was centrifuged (1500G, 3min) every week.After incubation for 0, 7, 14, 28, and 56 d, saline(NaCl 8.0 g/L, KCl 0.2 g/L) was added to the modelsoil. The model soil was sonicated for 20 sec, andmixed with a spatula.2.7 Measurement of Total Organic Carbon andSulfate ConcentrationsSulfate concentration and TOC concentration in theculture was measured by sulfur analyzer Antek (9000Series) and a TOC analyzer, respectively. The pH ofthe culture tenfold-diluted solution was measured bya pH meter. Corrosion products were selectivelyremoved from the corroded carbon steel coupons asdescribed above. The roughness of the coupon wasanalyzed by a laser 3D profile microscope (VK-8500).2.8 Bacterial countTo count the aerobes in the culture, saline was addedto the model soil and the supernatant was spread-plated on Minimized Luria-Bertani (MLB) agar plate,containing (in g/L) polypeptone 1.0, yeast extract 0.5,NaCl 10.0, and agar 15, in triplicate. Afterincubation for 7 d at 28oC, the observed colonieswere counted as aerobes. For the counting ofanaerobes and SRB in the experimental culture, thesupernatant was added dropwise to the plates and theMBM agar medium with 173 (in g/L)Fe(NH4)2(SO4)2 was poured. The plates wereincubated in sealed jars with an oxygen absorbingand carbon dioxide generating agent. Afterincubation for 14 d at 37oC, the observed black
Mataqi, K.Y. , Akbar, B.H. / International Journal of Engineering Research and Applications(IJERA) ISSN: 2248-9622 www.ijera.comVol. 3, Issue 2, March -April 2013, pp.617-623619 | P a g ecolonies were counted as SRB and others werecounted as anaerobes. The concentration of bacteriawas expressed as (CFU) per mL.III. Results3.1 Analysis of corroded carbon steelThe CMDs of carbon steel coupons underanaerobic and aerobic conditions were comparedafter 56 days incubation period. In Bacterialconsortia, the CMD under aerobic conditions reached34.1 µm, which was 28 times higher than anaerobicconditions with CMD measurement of only 1.2 µm.However, the CMD for SRB-inoculation or sterileconditions reached 5.42 or 5.11 µm respectively, inwhich was 8.9 or 8.8 times higher than the anaerobicconditions (Fig. 2A, Table 1). There weren’t anysignificant differences between SRB and sterilecontrol conditions, yet in Bacterial consortia achange was noted with 2.1 and 6.7 times increase inanaerobic and aerobic treatments respectively, whencompared with sterile CMD values. Theseobservations indicated that existence of oxygencauses carbon steel corrosion in model soil.Figure 2. Time Course of CMD (A), sulfateconcentration (B), TOC concentration (C) , and pH(D) under anaerobic ( , , , ) and aerobic ( , ,) conditions. The test was conducted in SRB culture( , ), bacterial consortia ( , ) and in sterileconditions as a control ( , ).Table 1. Effect of dissolved Oxygen Existence andBacteria on Endpoint CMD (µm) after 56 daysIncubationSRB BacterialconsortiaSterileAnaerobic 0.61 1.2 0.58Aerobic 5.42 34.1 5.11Upon inoculation of SRB under aerobic conditions,little corrosion on the steel coupons was observedduring the 14-28 days incubation period. In themodel soil analyzed, a gap separating the soil intoupper and lower parts was observed just afterincubation for 7 days. This gap seemed to influencecorrosion acceleration, as the coupons were corrodedunexpectedly at day 7. The whole surface of couponimmersed into the SRB culture was covered withhomogeneous black corrosion products that wereeasily wiped off. When the corroded coupons wereincubated with HCl, hydrogen sulfide (H2S) gas wasproduced, indicating that FeS was formed. Inaddition, local corrosion under black tubercles wasobserved under aerobic conditions. Theseobservations showed that the sole existence of SRBdidn`t accelerate carbon steel corrosion, while that ofBacterial consortia did indeed accelerate thecorrosion process.3.2 Influence of pH, Sulfate and TOC concentrationson bacterial growth over timeSulfate concentration for the SRB inoculated in bothanaerobic and aerobic conditions stopped decreasingat day 7 suggesting that the sulfate-reducing activityof SRB was high until this day as it began to decreaseafterwards. While, the sulfate concentration forBacterial consortia stopped decreasing at day 14(Fig. 2B). Incubation of carbon steel coupons withSRB or Bacterial consortia inoculae lead to thedepletion of TOC concentration at day 7;furthermore, heterotrophic bacteria were inactiveduring the 14-56 day incubation period (Fig. 2C) andthe concentration of aerobes decreased as well (Fig.3A). Under anaerobic conditions, the TOC was notconsumed completely, because oxygen as electronacceptor was limited. TOC concentration decreasedeven under sterile conditions. In another experimentwith sterile conditions that did not contain carbon
Mataqi, K.Y. , Akbar, B.H. / International Journal of Engineering Research and Applications(IJERA) ISSN: 2248-9622 www.ijera.comVol. 3, Issue 2, March -April 2013, pp.617-623620 | P a g esteel coupons, the TOC concentration however didnot decrease (data not shown). This indicates that thecorrosion products adsorbed the organic carbon.Under anaerobic conditions, SRB concentration wasdecreased and became negligible during the 28-56day incubation period (Fig. 3C). This is due to thefact that insufficient sulfate and hydrogen sulfide thatfilled the tested bottle inhibited the growth of SRB.Under aerobic conditions, the presence of SRBsuggested the formation of anaerobic regions in thesoil.When examining the pH concentration underanaerobic conditions, it increased to 7.9 afterincubation for 7 days and remained constant for 50days. On the other hand, the pH under aerobicconditions was slightly higher as it increased to 9after similar incubation time and remained constantfor 50 days as well (Fig. 2D). In SRB cultureincubated under both anaerobic and aerobicconditions, there was no detection of SRB during the28-56 day incubation period (Fig. 3C). In contrast,Bacterial consortia cell concentrations reached 108CFU/mL under aerobic conditions, while SRBreached just over 105CFU/mL, after incubation for28 days. As for the sulfate concentration, it remainedaround 1400mg/L throughout the experiment. Theincrease of SRB at 7 day incubation time indicatedthat SRB was not dormant and sulfate-reducingactivity occurred during this time. This observationsuggested that sulfur-oxidizing bacteria (SOB)generated sulfate and lived symbiotically with SRB,in addition to the oxidation of sulfide within thedissolved oxygen.Figure 3. Time course on the concentration ofaerobes (A), anearobes (B), and SRB (C). Incubationwas carried out under anaerobic ( , ) and aerobic( , ) conditions. , :In SRB culture, ,: In bacterial consortia. Cell concentrations weremeausred over a 60 day (d) period.3.3 Characteristic of SRB coloniesFor the counting of SRB in the culture of Bacterialconsortia, the culture broth was inoculated intoMBM agar plate under anaerobic condition. Afterincubation for 7 days, a black colony was observed inthe plate. Following this period, the entire platebecame black due to H2S produced from the SRBcolony. Clear zones surrounding the bacterialcolonies in the FeS on the MBM agar plates wereobserved (Fig. 4).
Mataqi, K.Y. , Akbar, B.H. / International Journal of Engineering Research and Applications(IJERA) ISSN: 2248-9622 www.ijera.comVol. 3, Issue 2, March -April 2013, pp.617-623621 | P a g eFigure 4. Clear zones surrounding the bacterialcolonies in the FeS on the MBM agar platesincubated under anaerobic conditions.3.4 Effects of Water Content on carbon steel couponsroughnessIn case of 60% WC, the boundary linebetween water phase and air phase was observed atthe center of the carbon steel coupons. Yet, for 20%WC, the boundary line was not observed on thecoupons. Examination of the eroded region on thecorroded coupon in terms of 60% WC, it was limitedto the lower half (Fig. 5C). On the other hand, in thecase of 20% WC, the eroded region was observedover the whole area on the coupons. Shiny metalsurfaces remained after incubation for 56 days (Fig.5D). In comparison with 100% WC, the erodedregion was observed over the entire coupon, anddeveloped pitting was observed (Fig. 5B). The CMDunder sterile conditions with 60% WC reached22.5µm and was 4.4 times higher than 100% WC(5.11µm) after incubation for 56 days (Fig. 6B, Table2). CMD was directly proportional to the incubationtime (R2= 0.993). CMD under sterile conditions with20% WC reached 30.0µm and was 5.9 times morethan 100% WC after incubation for 56 days. TheCMD was directly proportional to the incubation time(R2= 0.999).Figure 5. Surface roughness analysis of corrodedcarbon steel coupons immersed in bacterial consortiaunder 100, 60 and 20% WC conditions. Corrosionproducts were selectively removed and the roughnessof the metal surface was analyzed. The controlcoupon was immersed in sterile conditions. Under60% WC condition, the lower half of coupon waseluted. Under 20% WC condition, shiny metalsurfaces were observed.Figure 6. Time course of CMD in bacterial consortia
Mataqi, K.Y. , Akbar, B.H. / International Journal of Engineering Research and Applications(IJERA) ISSN: 2248-9622 www.ijera.comVol. 3, Issue 2, March -April 2013, pp.617-623622 | P a g e( , , ) and sterile conditions ( , , ) with100% WC ( , ), 60% WC ( , ), and 20%WC ( , ).Cell concentrations were meausred over a 60 day (d)period.Table 2. Effect of Water Content on Endpoint CMD(µm) after 56 days IncubationBacterialconsortiaSterile100% WC 34.1 5.1160% WC 35.9 22.520% WC 37.1 30.0Bacterial consortia accelerated the corrosion of thecarbon steel coupons under three WC conditions.CMDs in the cases of 100, 60 and 20% WC reached34.1, 35.9 and 37.1µm, respectively after incubationfor 56 days (Fig. 6A, Table 2). In the case of 100%WC, CMD was slightly increased until the 14thincubation day and the corrosion rate was acceleratedafter that. No distinct difference in CMD among thethree WC conditions was observed nor was there anydetection of SRB after incubation for 56 days. Theconcentrations of aerobes and anaerobes decreasedunder incubation with all three WC conditions (Fig.7).Figure 7. Time course of concentration of aerobes(A), anaerobes (B), and SRB (C). Incubation wascarried out under 100% WC ( ), 60% WC ( ), and20% WC ( ). Cell concentrations were meausredover a 60 day (d) period.IV. DiscussionAerobic conditions accelerated the corrosionof carbon steel in model soil. SRB inoculationinhibited the corrosion under aerobic conditions atday 14 and 28. The whole surfaces of the corrodedsteel coupons were covered with homogeneoussulfide (FeS). Ma et al. reported that corrosion of99.99% pure iron immersed in solution was inhibitedby a protective layer of FeS under such conditions asless than 0.04 mmol dm-3H2S concentration, a pHvalue of 3-5 and an immersion time longer than 2 h. When the entire coupon surface was coveredwith homogeneous ferrous sulfide, corrosion ofcarbon steel was inhibited. Under anaerobic oraerobic condition, sulfate concentration for the SRBinoculated condition stopped decreasing at day 7because of either the product (H2S) inhibition orlactate depletion, respectively. The observationunder anaerobic condition indicated that hydrogensulfide didn`t accelerate corrosion of carbon steel.Corrosion acceleration by SRB activity such as thecathodic depolarization was stopped at day 7.Bacterial consortia accelerated the corrosion ofcarbon steel. However, in the soil contained water,little convection occurred. Therefore, segregation ofbacterial habitat and uneven distribution of dissolvedoxygen in the culture were considered to be formedin the soil. It is indicated that the heterogeneousstructure led to the formation of a heterogeneousbiofilm with corrosion products on the carbon steelcoupons. The heterogeneous biofilm that resulted inthe uneven distribution of dissolved oxygen on themetal surface and the formation of oxygenconcentration cells accelerated microbial corrosion.Therefore, the heterogeneity caused acceleration inmodel soil. Dubiel et al. reported that the corrosionof carbon steel in the culture inoculated with bothSOB and SRB was accelerated compared to that inthe culture inoculated with either SOB or SRB .In our experiments, SRB colonies and FeS wereobserved on MBM agar plates inoculated withBacterial consortia culture. The entire plate becameblack due to H2S produced by the SRB colony. Clearzones surrounding the bacterial colonies in the FeSwere observed. On the carbon steel couponsimmersed into Bacterial consortia, the protective FeSfilm formed by SRB was broken by the bacteriaobserved in the clear zone. The bacteria wereconsidered to be SOB and the mechanism ofcorrosion was proposed in Fig. 8. That is being, (1)SRB generate H2S from sulfate, (2) carbon steelcoupons are protected by FeS, (3) SOB break theprotective FeS film and sulfate is generated.
Mataqi, K.Y. , Akbar, B.H. / International Journal of Engineering Research and Applications(IJERA) ISSN: 2248-9622 www.ijera.comVol. 3, Issue 2, March -April 2013, pp.617-623623 | P a g eFigure 8. Sulfur cycle with SRB and SOBaccelerating carbon steel corrosion.The corrosion rate of carbon steel couponsincreased in the order of 20, 60, and 100% WC. Inthe case of 60% WC, boundary line between thewater phase and the air phase was observed at thecenter of carbon steel coupons. Above the waterphase, the soil had adhering water. In the case of20% WC, corrosion that begun from adhering waterextended to cover the entire carbon steel coupons. Inthe case of 60% WC, the corrosion was observed noton the upper half of coupon but on the lower half.The difference in dissolved oxygen concentrationbetween the parts under adhering water and the metalsurface on the upper half of the coupon was less thanthat between the lower half and the upper half of thecoupons. Therefore, the oxygen concentration cellreaction was limited between the lower half and theupper half of the coupon. The uneven distribution ofwater and air spaces on the carbon steel couponsaccelerated the corrosion.In Bacteria consortia, the corrosion of carbon steelcoupons under 60 and 100% WC conditions wasaccelerated to almost same level as the corrosionobserved under the 20% WC condition. Therefore,the heterogeneity resulting from bacteria led to anuneven distribution of dissolved oxygen on thecarbon steel coupon, which is equal to thedistribution under the 20% WC condition, and thatwas the major mechanism of microbial corrosionacceleration.V. ConclusionCarbon steel coupons were immersed intoartificial model soil consisting of silica sand,microbes, and medium. Incubation was carried outunder anaerobic and aerobic conditions, and aerobicconditions were found to accelerate corrosion ofcarbon steel. Carbon steel coupons were immersedinto artificial model soils with 100, 60 and 20% WC.The existence of air space and the uneven distributionof medium on the carbon steel coupons acceleratedcorrosion. Sole SRB ceased the corrosion of carbonsteel with protective ferrous sulfide film. Unevendistribution of dissolved oxygen on the carbon steel,resulting from the heterogeneity of bacterial consortiahabitat, accelerated the corrosion of carbon steel.References S. Virtanen, I. Milosev, E. Gomez-Barrena, R.Trebse, J. Salo, and YT. Konttinen, Special modesof corrosion under physiological and simulatedphysiological conditions. Acta Biomater 4(3), 2008,468-76. R. B. Eckert, H. C. Aldrich, C. A. Edwards, B. A.Cookingham, Microscopic Differentiation of InternalCorrosion Initiation Mechanisms in Natural GasPipeline Systems. Corrosion, 2003, 1342-1355. R. Javaherdashti , Impact of sulphate-reducingbacteria on the performance of engineering materials.Appl Microbiol Biotechnology 91(6), 2011, 1507-17. A. G. Brooke, E.M. Watling, M. Attwood,M.&Tempest, D. W. Environmental Control ofMetabolic Fluxes in Thermotolerant MethylotrophicBacillus Strains. Archives of Microbiology. 151,1989, 268-273. RA . Lane, Under the microscope: understanding,detecting and preventing microbiologicallyinfluenced corrosion. AMPTIAC Quart 9(1), 2005,3–8. K. R. Butlin, M. E. Adams, and M. Thomas, Theisolation and cultivation of sulfate-reducing bacteria.J. Gen. Microbiology 3, 1949, 46-59. G.R. Gibson, Physiology and ecology of thesulphatereducing bacteria. J Appl Bacteriology 69,1990, 769–797. M.S. Wiener, B.V. Salas, M. Quintero-Nunez, andR. Zlatev. Effect of H2S on corrosion in pollutedwaters: a review. Corros. Eng. Sci. Technol. 41 (3),2006, 221–227. M. Magot, G. Ravot, X. Campaignolle, B. Ollivier,BKC. Patel , ML. Fardeau, P.Thomas, JL. Crolet, andJL. Garcia, Dethiosulfovibrio peptidovorans gen.nov., sp. nov., a new anaerobic, slightly halophilic,thiosulfate-reducing bacterium from corrodingoffshore oil wells. Int J Syst Bacteriol 47, 1997, 818–824. G.H. Koch, M. P. H. Brongers, N. G. Thompson, Y.P. Virmani, and J. H. Payer, Corrosion costs andpreventive strategies in the United States. 2001.FHWA-RD-01–156. [Online.] Federal HighwayAdministration, Washington,D.C.http://www.corrosioncost.com/. E. Rob, Biological corrosion of metals. FaliureAnalysis. 2010. [Online.] http://failure-analysis.info/2010/06/biological-corrosion-of-metals/. E.J. Akpabio, E.J . Ekott, and M.E. Akpan, Inhibitionand control of microbiologically influenced corrosionin oilfield materials. Environmental ResearchJournal 5(2), 2011, 59-65. H. Ma, X. Cheng, S. Li, Z. Chen, S. Quan, L. Zhao,and S. Niu, Corrosion Science. 42, 2000, 1669-1683. M. Dubiel, C. H. Hsu, C. C. Chien, F. Mansfeld, andD.K. Newman, Microbial Iron Respiration CanProtect Steel from Corrosion. Applied andEnvironmental Microbiology 68, 2002,1440-1445.